#------------------------------------------------------------------------------
#$Date: 2016-03-26 19:23:19 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180432 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/01/7210129.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7210129
loop_
_publ_author_name
'Chen, Zhaofei'
'An, Haiyan'
'Zhang, Hua'
'Hu, Ying'
_publ_section_title
;
 Metal(ii)-directed self-assembly of amino acid functionalized
 polyoxometalates
;
_journal_issue                   23
_journal_name_full               CrystEngComm
_journal_page_first              4711
_journal_paper_doi               10.1039/c3ce40129d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C12 H50 Mo8 N4 O40 Zn'
_chemical_formula_weight         1723.47
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                117.5610(10)
_cell_angle_beta                 90.0820(10)
_cell_angle_gamma                110.5770(10)
_cell_formula_units_Z            1
_cell_length_a                   9.7735(3)
_cell_length_b                   11.6942(4)
_cell_length_c                   12.0719(4)
_cell_measurement_reflns_used    8950
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.94
_cell_volume                     1122.53(7)
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0202
_diffrn_reflns_av_sigmaI/netI    0.0245
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            8950
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.94
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.798
_exptl_absorpt_correction_T_max  0.588
_exptl_absorpt_correction_T_min  0.516
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.549
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             836
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.19
_refine_diff_density_max         1.515
_refine_diff_density_min         -0.864
_refine_diff_density_rms         0.150
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.153
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     313
_refine_ls_number_reflns         3947
_refine_ls_number_restraints     30
_refine_ls_restrained_S_all      1.168
_refine_ls_R_factor_all          0.0357
_refine_ls_R_factor_gt           0.0343
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0328P)²+6.5737P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0895
_refine_ls_wR_factor_ref         0.0903
_reflns_number_gt                3776
_reflns_number_total             3947
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce40129d.txt
_cod_data_source_block           5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        1122.53(6)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7210129
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.65605(5) 0.46802(5) 0.00951(4) 0.01925(13) Uani 1 1 d .
Mo2 Mo 0.73011(6) 0.80897(5) 0.25323(5) 0.02486(14) Uani 1 1 d .
Mo3 Mo 0.45513(5) 0.54780(5) 0.25296(5) 0.02333(14) Uani 1 1 d .
Mo4 Mo 0.10633(5) 0.24306(5) -0.00612(5) 0.02371(13) Uani 1 1 d .
Zn1 Zn 0.5000 0.0000 0.0000 0.0326(2) Uani 1 2 d S
O1 O 0.7452(5) 0.3593(4) -0.0670(4) 0.0300(9) Uani 1 1 d .
O2 O 0.8132(4) 0.6429(4) 0.1184(4) 0.0243(8) Uani 1 1 d .
O3 O 0.5288(4) 0.6212(4) 0.1108(3) 0.0206(8) Uani 1 1 d .
O4 O 0.5856(4) 0.4202(4) 0.1227(4) 0.0254(8) Uani 1 1 d .
O5 O 0.7769(4) 0.8469(4) 0.1129(4) 0.0270(9) Uani 1 1 d .
O6 O 0.8996(5) 0.9031(5) 0.3530(4) 0.0422(11) Uani 1 1 d .
O7 O 0.6297(6) 0.9127(5) 0.3113(5) 0.0418(11) Uani 1 1 d .
O8 O 0.6564(4) 0.6840(4) 0.3227(4) 0.0284(9) Uani 1 1 d .
O9 O 0.3663(5) 0.6567(5) 0.3335(4) 0.0385(11) Uani 1 1 d .
O10 O 0.4369(5) 0.4481(5) 0.3241(4) 0.0398(11) Uani 1 1 d .
O11 O 0.3084(4) 0.4240(4) 0.0970(4) 0.0247(8) Uani 1 1 d .
O12 O -0.0648(5) 0.1527(5) -0.1057(5) 0.0406(11) Uani 1 1 d .
O13 O 0.0955(5) 0.1774(5) 0.0933(4) 0.0380(11) Uani 1 1 d .
O14 O 0.0399(5) 0.4065(5) 0.1105(4) 0.0345(10) Uani 1 1 d .
O15 O -0.1251(6) 0.3139(5) 0.2050(6) 0.0541(14) Uani 1 1 d .
C1 C -0.0390(7) 0.4127(7) 0.1959(6) 0.0318(14) Uani 1 1 d .
C2 C -0.0111(11) 0.5620(8) 0.2980(8) 0.061(2) Uani 1 1 d U
C3 C -0.0890(17) 0.5935(17) 0.3963(15) 0.044(3) Uani 0.50 1 d P
C3A C 0.0226(16) 0.5984(14) 0.4263(11) 0.035(3) Uani 0.50 1 d P
C4 C 0.0079(10) 0.7384(9) 0.5268(8) 0.058(2) Uani 1 1 d .
C5 C -0.1310(15) 0.7252(14) 0.5822(13) 0.098(4) Uani 1 1 d U
H5A H -0.2144 0.6516 0.5131 0.118 Uiso 1 1 calc R
H5B H -0.1238 0.6921 0.6414 0.118 Uiso 1 1 calc R
C6 C -0.1682(15) 0.8408(13) 0.6451(12) 0.096(4) Uani 1 1 d U
H6A H -0.2004 0.8568 0.5794 0.115 Uiso 1 1 calc R
H6B H -0.0754 0.9203 0.6956 0.115 Uiso 1 1 calc R
N1 N 0.0587(5) 0.6624(5) 0.2534(5) 0.0284(11) Uani 1 1 d .
H1A H 0.0739 0.7488 0.3145 0.043 Uiso 1 1 calc R
H1B H -0.0009 0.6402 0.1845 0.043 Uiso 1 1 calc R
H1C H 0.1456 0.6590 0.2341 0.043 Uiso 1 1 calc R
N2 N -0.2731(8) 0.8526(8) 0.7257(7) 0.0619(19) Uani 1 1 d .
H2A H -0.2805 0.9347 0.7526 0.093 Uiso 1 1 calc R
H2B H -0.2434 0.8476 0.7925 0.093 Uiso 1 1 calc R
H2C H -0.3615 0.7829 0.6829 0.093 Uiso 1 1 calc R
O1W O 0.7142(5) 0.0246(5) 0.0542(6) 0.0527(14) Uani 1 1 d .
O2W O 0.4211(6) -0.0784(5) 0.1287(5) 0.0498(13) Uani 1 1 d .
O3W O 0.5408(6) 0.1968(5) 0.1520(5) 0.0479(13) Uani 1 1 d .
O4W O 0.3140(8) 0.9205(7) 0.4120(6) 0.085(2) Uani 1 1 d .
O5W O 0.581(2) 0.309(2) 0.4135(16) 0.103(5) Uani 0.50 1 d PU
O6W O 0.551(2) 0.172(2) 0.3940(17) 0.113(6) Uani 0.50 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Mo1 O4 103.99(19) . .
O1 Mo1 O2 103.78(19) . .
O4 Mo1 O2 99.75(18) . .
O1 Mo1 O3 102.15(18) . 2_665
O4 Mo1 O3 98.10(17) . 2_665
O2 Mo1 O3 143.72(16) . 2_665
O1 Mo1 O11 98.83(18) . 2_665
O4 Mo1 O11 157.09(17) . 2_665
O2 Mo1 O11 76.44(15) . 2_665
O3 Mo1 O11 74.87(15) 2_665 2_665
O1 Mo1 O3 178.08(17) . .
O4 Mo1 O3 77.67(15) . .
O2 Mo1 O3 76.76(15) . .
O3 Mo1 O3 76.58(15) 2_665 .
O11 Mo1 O3 79.48(14) 2_665 .
O1 Mo1 Mo3 91.58(15) . 2_665
O4 Mo1 Mo3 140.96(13) . 2_665
O2 Mo1 Mo3 111.12(12) . 2_665
O3 Mo1 Mo3 43.14(11) 2_665 2_665
O11 Mo1 Mo3 34.70(10) 2_665 2_665
O3 Mo1 Mo3 86.52(9) . 2_665
O1 Mo1 Mo4 98.03(14) . 2_665
O4 Mo1 Mo4 138.06(13) . 2_665
O2 Mo1 Mo4 39.74(12) . 2_665
O3 Mo1 Mo4 111.66(11) 2_665 2_665
O11 Mo1 Mo4 37.59(10) 2_665 2_665
O3 Mo1 Mo4 81.19(9) . 2_665
Mo3 Mo1 Mo4 72.063(15) 2_665 2_665
O1 Mo1 Mo1 145.37(15) . 2_665
O4 Mo1 Mo1 85.94(13) . 2_665
O2 Mo1 Mo1 107.11(12) . 2_665
O3 Mo1 Mo1 43.24(11) 2_665 2_665
O11 Mo1 Mo1 73.97(10) 2_665 2_665
O3 Mo1 Mo1 33.34(9) . 2_665
Mo3 Mo1 Mo1 62.931(16) 2_665 2_665
Mo4 Mo1 Mo1 95.775(19) 2_665 2_665
O6 Mo2 O7 105.9(2) . .
O6 Mo2 O8 94.8(2) . .
O7 Mo2 O8 101.5(2) . .
O6 Mo2 O5 100.6(2) . .
O7 Mo2 O5 95.7(2) . .
O8 Mo2 O5 152.76(17) . .
O6 Mo2 O3 159.5(2) . .
O7 Mo2 O3 92.65(19) . .
O8 Mo2 O3 72.61(15) . .
O5 Mo2 O3 85.78(15) . .
O6 Mo2 O2 90.3(2) . .
O7 Mo2 O2 162.13(19) . .
O8 Mo2 O2 84.01(16) . .
O5 Mo2 O2 73.62(15) . .
O3 Mo2 O2 72.62(13) . .
O6 Mo2 Mo3 126.14(16) . .
O7 Mo2 Mo3 89.81(16) . .
O8 Mo2 Mo3 31.37(12) . .
O5 Mo2 Mo3 129.30(12) . .
O3 Mo2 Mo3 43.57(9) . .
O2 Mo2 Mo3 86.32(10) . .
O6 Mo2 Mo4 90.15(17) . 2_665
O7 Mo2 Mo4 127.07(17) . 2_665
O8 Mo2 Mo4 127.50(12) . 2_665
O5 Mo2 Mo4 31.34(12) . 2_665
O3 Mo2 Mo4 85.27(9) . 2_665
O2 Mo2 Mo4 43.65(10) . 2_665
Mo3 Mo2 Mo4 120.684(18) . 2_665
O10 Mo3 O9 104.9(2) . .
O10 Mo3 O8 103.4(2) . .
O9 Mo3 O8 98.2(2) . .
O10 Mo3 O11 103.9(2) . .
O9 Mo3 O11 98.1(2) . .
O8 Mo3 O11 143.11(17) . .
O10 Mo3 O3 155.70(19) . .
O9 Mo3 O3 99.44(19) . .
O8 Mo3 O3 72.87(15) . .
O11 Mo3 O3 71.95(15) . .
O10 Mo3 O4 85.23(19) . .
O9 Mo3 O4 169.90(19) . .
O8 Mo3 O4 78.85(16) . .
O11 Mo3 O4 79.31(15) . .
O3 Mo3 O4 70.47(13) . .
O10 Mo3 Mo1 142.62(16) . 2_665
O9 Mo3 Mo1 89.93(16) . 2_665
O8 Mo3 Mo1 108.21(12) . 2_665
O11 Mo3 Mo1 39.16(11) . 2_665
O3 Mo3 Mo1 35.65(9) . 2_665
O4 Mo3 Mo1 81.93(10) . 2_665
O10 Mo3 Mo2 135.00(16) . .
O9 Mo3 Mo2 90.92(16) . .
O8 Mo3 Mo2 31.77(12) . .
O11 Mo3 Mo2 115.34(12) . .
O3 Mo3 Mo2 43.45(9) . .
O4 Mo3 Mo2 81.51(9) . .
Mo1 Mo3 Mo2 77.350(16) 2_665 .
O13 Mo4 O12 105.7(2) . .
O13 Mo4 O5 98.4(2) . 2_665
O12 Mo4 O5 101.6(2) . 2_665
O13 Mo4 O14 96.0(2) . .
O12 Mo4 O14 89.8(2) . .
O5 Mo4 O14 158.42(17) 2_665 .
O13 Mo4 O11 97.44(19) . .
O12 Mo4 O11 153.4(2) . .
O5 Mo4 O11 87.55(16) 2_665 .
O14 Mo4 O11 74.66(16) . .
O13 Mo4 O2 164.74(19) . 2_665
O12 Mo4 O2 89.15(19) . 2_665
O5 Mo4 O2 74.85(15) 2_665 2_665
O14 Mo4 O2 87.20(16) . 2_665
O11 Mo4 O2 68.98(14) . 2_665
O13 Mo4 Mo2 130.47(16) . 2_665
O12 Mo4 Mo2 90.11(16) . 2_665
O5 Mo4 Mo2 32.12(12) 2_665 2_665
O14 Mo4 Mo2 131.34(12) . 2_665
O11 Mo4 Mo2 84.55(11) . 2_665
O2 Mo4 Mo2 44.14(10) 2_665 2_665
O13 Mo4 Mo1 135.09(16) . 2_665
O12 Mo4 Mo1 117.71(17) . 2_665
O5 Mo4 Mo1 84.22(12) 2_665 2_665
O14 Mo4 Mo1 74.24(12) . 2_665
O11 Mo4 Mo1 37.68(10) . 2_665
O2 Mo4 Mo1 32.07(9) 2_665 2_665
Mo2 Mo4 Mo1 63.077(14) 2_665 2_665
O3W Zn1 O3W 180.0(5) . 2_655
O3W Zn1 O1W 90.2(2) . 2_655
O3W Zn1 O1W 89.8(2) 2_655 2_655
O3W Zn1 O1W 89.8(2) . .
O3W Zn1 O1W 90.2(2) 2_655 .
O1W Zn1 O1W 180.0(3) 2_655 .
O3W Zn1 O2W 94.01(19) . 2_655
O3W Zn1 O2W 85.99(19) 2_655 2_655
O1W Zn1 O2W 90.5(2) 2_655 2_655
O1W Zn1 O2W 89.5(2) . 2_655
O3W Zn1 O2W 85.99(19) . .
O3W Zn1 O2W 94.01(19) 2_655 .
O1W Zn1 O2W 89.5(2) 2_655 .
O1W Zn1 O2W 90.5(2) . .
O2W Zn1 O2W 180.0(2) 2_655 .
Mo1 O2 Mo4 108.19(17) . 2_665
Mo1 O2 Mo2 112.76(18) . .
Mo4 O2 Mo2 92.21(14) 2_665 .
Mo1 O3 Mo2 153.70(19) 2_665 .
Mo1 O3 Mo3 101.21(15) 2_665 .
Mo2 O3 Mo3 92.98(14) . .
Mo1 O3 Mo1 103.42(15) 2_665 .
Mo2 O3 Mo1 96.79(13) . .
Mo3 O3 Mo1 96.36(13) . .
Mo1 O4 Mo3 115.46(19) . .
Mo4 O5 Mo2 116.5(2) 2_665 .
Mo3 O8 Mo2 116.9(2) . .
Mo3 O11 Mo4 148.0(2) . .
Mo3 O11 Mo1 106.14(17) . 2_665
Mo4 O11 Mo1 104.73(16) . 2_665
C1 O14 Mo4 128.2(4) . .
O15 C1 O14 126.8(6) . .
O15 C1 C2 119.5(6) . .
O14 C1 C2 113.6(6) . .
C3 C2 C3A 47.4(9) . .
C3 C2 N1 121.3(9) . .
C3A C2 N1 121.7(8) . .
C3 C2 C1 123.4(9) . .
C3A C2 C1 117.9(8) . .
N1 C2 C1 111.1(6) . .
C3A C3 C2 67.4(10) . .
C3A C3 C4 67.3(11) . .
C2 C3 C4 113.7(11) . .
C3 C3A C2 65.2(10) . .
C3 C3A C4 71.8(11) . .
C2 C3A C4 115.2(10) . .
C5 C4 C3A 117.8(9) . .
C5 C4 C3 89.0(9) . .
C3A C4 C3 40.9(7) . .
C6 C5 C4 120.3(11) . .
C6 C5 H5A 107.2 . .
C4 C5 H5A 107.2 . .
C6 C5 H5B 107.2 . .
C4 C5 H5B 107.2 . .
H5A C5 H5B 106.9 . .
C5 C6 N2 125.7(11) . .
C5 C6 H6A 105.9 . .
N2 C6 H6A 105.9 . .
C5 C6 H6B 105.9 . .
N2 C6 H6B 105.9 . .
H6A C6 H6B 106.2 . .
C2 N1 H1A 109.5 . .
C2 N1 H1B 109.5 . .
H1A N1 H1B 109.5 . .
C2 N1 H1C 109.5 . .
H1A N1 H1C 109.5 . .
H1B N1 H1C 109.5 . .
C6 N2 H2A 109.5 . .
C6 N2 H2B 109.5 . .
H2A N2 H2B 109.5 . .
C6 N2 H2C 109.5 . .
H2A N2 H2C 109.5 . .
H2B N2 H2C 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O1 1.709(4) .
Mo1 O4 1.758(4) .
Mo1 O2 1.889(4) .
Mo1 O3 1.931(4) 2_665
Mo1 O11 2.136(4) 2_665
Mo1 O3 2.407(4) .
Mo1 Mo3 3.2497(7) 2_665
Mo1 Mo4 3.3799(6) 2_665
Mo1 Mo1 3.4172(9) 2_665
Mo2 O6 1.701(4) .
Mo2 O7 1.725(4) .
Mo2 O8 1.937(4) .
Mo2 O5 1.957(4) .
Mo2 O3 2.260(4) .
Mo2 O2 2.295(4) .
Mo2 Mo3 3.2821(7) .
Mo2 Mo4 3.2928(7) 2_665
Mo3 O10 1.706(4) .
Mo3 O9 1.719(4) .
Mo3 O8 1.915(4) .
Mo3 O11 1.926(4) .
Mo3 O3 2.265(4) .
Mo3 O4 2.344(4) .
Mo3 Mo1 3.2497(7) 2_665
Mo4 O13 1.685(4) .
Mo4 O12 1.713(4) .
Mo4 O5 1.915(4) 2_665
Mo4 O14 2.108(4) .
Mo4 O11 2.132(4) .
Mo4 O2 2.275(4) 2_665
Mo4 Mo2 3.2928(7) 2_665
Mo4 Mo1 3.3799(6) 2_665
Zn1 O3W 2.066(5) .
Zn1 O3W 2.066(5) 2_655
Zn1 O1W 2.072(5) 2_655
Zn1 O1W 2.072(5) .
Zn1 O2W 2.162(5) 2_655
Zn1 O2W 2.162(5) .
O2 Mo4 2.275(4) 2_665
O3 Mo1 1.931(4) 2_665
O5 Mo4 1.915(4) 2_665
O11 Mo1 2.136(4) 2_665
O14 C1 1.279(8) .
O15 C1 1.220(8) .
C1 C2 1.522(10) .
C2 C3 1.385(15) .
C2 C3A 1.407(14) .
C2 N1 1.469(9) .
C3 C3A 1.122(19) .
C3 C4 1.627(19) .
C3A C4 1.581(15) .
C4 C5 1.506(14) .
C5 C6 1.390(15) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 N2 1.412(11) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
N1 H1A 0.8900 .
N1 H1B 0.8900 .
N1 H1C 0.8900 .
N2 H2A 0.8900 .
N2 H2B 0.8900 .
N2 H2C 0.8900 .
O5W O6W 1.43(2) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O6 Mo2 Mo3 O10 -11.3(3) . .
O7 Mo2 Mo3 O10 -121.0(3) . .
O8 Mo2 Mo3 O10 -8.1(3) . .
O5 Mo2 Mo3 O10 141.7(3) . .
O3 Mo2 Mo3 O10 144.9(3) . .
O2 Mo2 Mo3 O10 76.4(3) . .
Mo4 Mo2 Mo3 O10 104.7(2) 2_665 .
O6 Mo2 Mo3 O9 101.0(3) . .
O7 Mo2 Mo3 O9 -8.7(2) . .
O8 Mo2 Mo3 O9 104.2(3) . .
O5 Mo2 Mo3 O9 -106.0(2) . .
O3 Mo2 Mo3 O9 -102.8(2) . .
O2 Mo2 Mo3 O9 -171.29(19) . .
Mo4 Mo2 Mo3 O9 -143.08(16) 2_665 .
O6 Mo2 Mo3 O8 -3.2(3) . .
O7 Mo2 Mo3 O8 -112.9(3) . .
O5 Mo2 Mo3 O8 149.8(3) . .
O3 Mo2 Mo3 O8 153.0(3) . .
O2 Mo2 Mo3 O8 84.5(3) . .
Mo4 Mo2 Mo3 O8 112.7(2) 2_665 .
O6 Mo2 Mo3 O11 -159.6(3) . .
O7 Mo2 Mo3 O11 90.7(2) . .
O8 Mo2 Mo3 O11 -156.4(3) . .
O5 Mo2 Mo3 O11 -6.5(2) . .
O3 Mo2 Mo3 O11 -3.35(19) . .
O2 Mo2 Mo3 O11 -71.85(16) . .
Mo4 Mo2 Mo3 O11 -43.64(13) 2_665 .
O6 Mo2 Mo3 O3 -156.2(3) . .
O7 Mo2 Mo3 O3 94.1(2) . .
O8 Mo2 Mo3 O3 -153.0(3) . .
O5 Mo2 Mo3 O3 -3.2(2) . .
O2 Mo2 Mo3 O3 -68.49(16) . .
Mo4 Mo2 Mo3 O3 -40.28(13) 2_665 .
O6 Mo2 Mo3 O4 -85.7(2) . .
O7 Mo2 Mo3 O4 164.5(2) . .
O8 Mo2 Mo3 O4 -82.5(3) . .
O5 Mo2 Mo3 O4 67.30(18) . .
O3 Mo2 Mo3 O4 70.50(16) . .
O2 Mo2 Mo3 O4 2.00(13) . .
Mo4 Mo2 Mo3 O4 30.21(10) 2_665 .
O6 Mo2 Mo3 Mo1 -169.3(2) . 2_665
O7 Mo2 Mo3 Mo1 80.97(17) . 2_665
O8 Mo2 Mo3 Mo1 -166.1(2) . 2_665
O5 Mo2 Mo3 Mo1 -16.27(15) . 2_665
O3 Mo2 Mo3 Mo1 -13.08(13) . 2_665
O2 Mo2 Mo3 Mo1 -81.57(9) . 2_665
Mo4 Mo2 Mo3 Mo1 -53.36(2) 2_665 2_665
O1 Mo1 O2 Mo4 86.0(2) . 2_665
O4 Mo1 O2 Mo4 -166.87(18) . 2_665
O3 Mo1 O2 Mo4 -48.5(3) 2_665 2_665
O11 Mo1 O2 Mo4 -9.94(16) 2_665 2_665
O3 Mo1 O2 Mo4 -92.11(17) . 2_665
Mo3 Mo1 O2 Mo4 -11.19(19) 2_665 2_665
Mo1 Mo1 O2 Mo4 -78.14(16) 2_665 2_665
O1 Mo1 O2 Mo2 -173.53(19) . .
O4 Mo1 O2 Mo2 -66.4(2) . .
O3 Mo1 O2 Mo2 52.0(3) 2_665 .
O11 Mo1 O2 Mo2 90.53(19) 2_665 .
O3 Mo1 O2 Mo2 8.36(15) . .
Mo3 Mo1 O2 Mo2 89.29(16) 2_665 .
Mo4 Mo1 O2 Mo2 100.5(2) 2_665 .
Mo1 Mo1 O2 Mo2 22.33(19) 2_665 .
O6 Mo2 O2 Mo1 159.3(2) . .
O7 Mo2 O2 Mo1 -44.7(7) . .
O8 Mo2 O2 Mo1 64.5(2) . .
O5 Mo2 O2 Mo1 -99.8(2) . .
O3 Mo2 O2 Mo1 -9.09(17) . .
Mo3 Mo2 O2 Mo1 33.13(16) . .
Mo4 Mo2 O2 Mo1 -110.8(2) 2_665 .
O6 Mo2 O2 Mo4 -89.88(19) . 2_665
O7 Mo2 O2 Mo4 66.1(6) . 2_665
O8 Mo2 O2 Mo4 175.32(16) . 2_665
O5 Mo2 O2 Mo4 11.04(14) . 2_665
O3 Mo2 O2 Mo4 101.70(14) . 2_665
Mo3 Mo2 O2 Mo4 143.92(10) . 2_665
O6 Mo2 O3 Mo1 -168.6(5) . 2_665
O7 Mo2 O3 Mo1 36.1(5) . 2_665
O8 Mo2 O3 Mo1 137.3(5) . 2_665
O5 Mo2 O3 Mo1 -59.5(4) . 2_665
O2 Mo2 O3 Mo1 -133.6(5) . 2_665
Mo3 Mo2 O3 Mo1 123.0(5) . 2_665
Mo4 Mo2 O3 Mo1 -90.9(4) 2_665 2_665
O6 Mo2 O3 Mo3 68.4(6) . .
O7 Mo2 O3 Mo3 -86.93(19) . .
O8 Mo2 O3 Mo3 14.33(15) . .
O5 Mo2 O3 Mo3 177.52(15) . .
O2 Mo2 O3 Mo3 103.38(15) . .
Mo4 Mo2 O3 Mo3 146.09(10) 2_665 .
O6 Mo2 O3 Mo1 -28.3(6) . .
O7 Mo2 O3 Mo1 176.30(19) . .
O8 Mo2 O3 Mo1 -82.44(16) . .
O5 Mo2 O3 Mo1 80.76(15) . .
O2 Mo2 O3 Mo1 6.61(12) . .
Mo3 Mo2 O3 Mo1 -96.77(15) . .
Mo4 Mo2 O3 Mo1 49.32(9) 2_665 .
O10 Mo3 O3 Mo1 103.0(5) . 2_665
O9 Mo3 O3 Mo1 -76.5(2) . 2_665
O8 Mo3 O3 Mo1 -172.2(2) . 2_665
O11 Mo3 O3 Mo1 19.07(16) . 2_665
O4 Mo3 O3 Mo1 103.83(17) . 2_665
Mo2 Mo3 O3 Mo1 -157.7(2) . 2_665
O10 Mo3 O3 Mo2 -99.2(5) . .
O9 Mo3 O3 Mo2 81.27(19) . .
O8 Mo3 O3 Mo2 -14.48(15) . .
O11 Mo3 O3 Mo2 176.81(18) . .
O4 Mo3 O3 Mo2 -98.43(15) . .
Mo1 Mo3 O3 Mo2 157.7(2) 2_665 .
O10 Mo3 O3 Mo1 -2.1(5) . .
O9 Mo3 O3 Mo1 178.45(17) . .
O8 Mo3 O3 Mo1 82.70(16) . .
O11 Mo3 O3 Mo1 -86.01(16) . .
O4 Mo3 O3 Mo1 -1.25(12) . .
Mo1 Mo3 O3 Mo1 -105.08(18) 2_665 .
Mo2 Mo3 O3 Mo1 97.18(15) . .
O1 Mo1 O3 Mo1 49(5) . 2_665
O4 Mo1 O3 Mo1 -101.56(19) . 2_665
O2 Mo1 O3 Mo1 155.2(2) . 2_665
O3 Mo1 O3 Mo1 0.0 2_665 2_665
O11 Mo1 O3 Mo1 76.78(17) 2_665 2_665
Mo3 Mo1 O3 Mo1 42.52(13) 2_665 2_665
Mo4 Mo1 O3 Mo1 114.89(14) 2_665 2_665
O1 Mo1 O3 Mo2 -114(5) . .
O4 Mo1 O3 Mo2 95.39(17) . .
O2 Mo1 O3 Mo2 -7.88(14) . .
O3 Mo1 O3 Mo2 -163.1(2) 2_665 .
O11 Mo1 O3 Mo2 -86.28(14) 2_665 .
Mo3 Mo1 O3 Mo2 -120.54(11) 2_665 .
Mo4 Mo1 O3 Mo2 -48.17(10) 2_665 .
Mo1 Mo1 O3 Mo2 -163.1(2) 2_665 .
O1 Mo1 O3 Mo3 152(5) . .
O4 Mo1 O3 Mo3 1.61(15) . .
O2 Mo1 O3 Mo3 -101.66(16) . .
O3 Mo1 O3 Mo3 103.16(18) 2_665 .
O11 Mo1 O3 Mo3 179.95(15) 2_665 .
Mo3 Mo1 O3 Mo3 145.68(11) 2_665 .
Mo4 Mo1 O3 Mo3 -141.94(11) 2_665 .
Mo1 Mo1 O3 Mo3 103.16(18) 2_665 .
O1 Mo1 O4 Mo3 179.3(2) . .
O2 Mo1 O4 Mo3 72.3(2) . .
O3 Mo1 O4 Mo3 -76.0(2) 2_665 .
O11 Mo1 O4 Mo3 -5.9(5) 2_665 .
O3 Mo1 O4 Mo3 -1.71(16) . .
Mo3 Mo1 O4 Mo3 -70.1(3) 2_665 .
Mo4 Mo1 O4 Mo3 59.7(3) 2_665 .
Mo1 Mo1 O4 Mo3 -34.38(16) 2_665 .
O10 Mo3 O4 Mo1 -178.5(2) . .
O9 Mo3 O4 Mo1 0.2(11) . .
O8 Mo3 O4 Mo1 -73.7(2) . .
O11 Mo3 O4 Mo1 76.4(2) . .
O3 Mo3 O4 Mo1 1.88(18) . .
Mo1 Mo3 O4 Mo1 36.74(18) 2_665 .
Mo2 Mo3 O4 Mo1 -41.58(18) . .
O6 Mo2 O5 Mo4 72.5(3) . 2_665
O7 Mo2 O5 Mo4 179.9(2) . 2_665
O8 Mo2 O5 Mo4 -50.8(5) . 2_665
O3 Mo2 O5 Mo4 -87.8(2) . 2_665
O2 Mo2 O5 Mo4 -14.72(19) . 2_665
Mo3 Mo2 O5 Mo4 -85.6(2) . 2_665
O10 Mo3 O8 Mo2 174.1(2) . .
O9 Mo3 O8 Mo2 -78.3(3) . .
O11 Mo3 O8 Mo2 37.1(4) . .
O3 Mo3 O8 Mo2 19.06(19) . .
O4 Mo3 O8 Mo2 91.9(2) . .
Mo1 Mo3 O8 Mo2 14.3(2) 2_665 .
O6 Mo2 O8 Mo3 177.4(3) . .
O7 Mo2 O8 Mo3 70.0(3) . .
O5 Mo2 O8 Mo3 -58.2(5) . .
O3 Mo2 O8 Mo3 -19.13(19) . .
O2 Mo2 O8 Mo3 -92.8(2) . .
Mo4 Mo2 O8 Mo3 -88.7(2) 2_665 .
O10 Mo3 O11 Mo4 22.8(4) . .
O9 Mo3 O11 Mo4 -84.8(4) . .
O8 Mo3 O11 Mo4 159.7(3) . .
O3 Mo3 O11 Mo4 177.9(4) . .
O4 Mo3 O11 Mo4 105.1(4) . .
Mo1 Mo3 O11 Mo4 -164.6(5) 2_665 .
Mo2 Mo3 O11 Mo4 -179.7(3) . .
O10 Mo3 O11 Mo1 -172.6(2) . 2_665
O9 Mo3 O11 Mo1 79.8(2) . 2_665
O8 Mo3 O11 Mo1 -35.7(4) . 2_665
O3 Mo3 O11 Mo1 -17.55(15) . 2_665
O4 Mo3 O11 Mo1 -90.32(17) . 2_665
Mo2 Mo3 O11 Mo1 -15.1(2) . 2_665
O13 Mo4 O11 Mo3 -13.5(4) . .
O12 Mo4 O11 Mo3 137.0(4) . .
O5 Mo4 O11 Mo3 -111.6(4) 2_665 .
O14 Mo4 O11 Mo3 80.7(4) . .
O2 Mo4 O11 Mo3 173.7(4) 2_665 .
Mo2 Mo4 O11 Mo3 -143.7(4) 2_665 .
Mo1 Mo4 O11 Mo3 164.7(5) 2_665 .
O13 Mo4 O11 Mo1 -178.2(2) . 2_665
O12 Mo4 O11 Mo1 -27.6(5) . 2_665
O5 Mo4 O11 Mo1 83.71(18) 2_665 2_665
O14 Mo4 O11 Mo1 -83.93(19) . 2_665
O2 Mo4 O11 Mo1 9.00(14) 2_665 2_665
Mo2 Mo4 O11 Mo1 51.65(13) 2_665 2_665
O13 Mo4 O14 C1 -24.9(5) . .
O12 Mo4 O14 C1 80.9(5) . .
O5 Mo4 O14 C1 -156.5(5) 2_665 .
O11 Mo4 O14 C1 -120.9(5) . .
O2 Mo4 O14 C1 170.1(5) 2_665 .
Mo2 Mo4 O14 C1 170.9(4) 2_665 .
Mo1 Mo4 O14 C1 -160.1(5) 2_665 .
Mo4 O14 C1 O15 -21.6(10) . .
Mo4 O14 C1 C2 154.9(5) . .
O15 C1 C2 C3 -6.2(15) . .
O14 C1 C2 C3 177.0(11) . .
O15 C1 C2 C3A 49.1(13) . .
O14 C1 C2 C3A -127.7(10) . .
O15 C1 C2 N1 -163.6(7) . .
O14 C1 C2 N1 19.7(10) . .
N1 C2 C3 C3A -106.0(13) . .
C1 C2 C3 C3A 98.9(13) . .
C3A C2 C3 C4 50.3(11) . .
N1 C2 C3 C4 -55.7(15) . .
C1 C2 C3 C4 149.2(9) . .
C4 C3 C3A C2 -130.2(9) . .
C2 C3 C3A C4 130.2(9) . .
N1 C2 C3A C3 105.2(13) . .
C1 C2 C3A C3 -111.1(12) . .
C3 C2 C3A C4 -53.3(12) . .
N1 C2 C3A C4 51.9(15) . .
C1 C2 C3A C4 -164.4(8) . .
C3 C3A C4 C5 50.3(13) . .
C2 C3A C4 C5 100.3(13) . .
C2 C3A C4 C3 50.0(11) . .
C3A C3 C4 C5 -137.1(11) . .
C2 C3 C4 C5 172.6(11) . .
C2 C3 C4 C3A -50.3(11) . .
C3A C4 C5 C6 -164.0(12) . .
C3 C4 C5 C6 -133.7(14) . .
C4 C5 C6 N2 -164.4(12) . .
